DOI: 10.17188/1679873
title: Materials Data on Li6MnV3(PO4)6 by Materials Project

description: Li6V3Mn(PO4)6 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Li–O bond distances ranging from 2.08–2.68 Å. In the second Li1+ site, Li1+ is bonded in a 3-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.96–2.64 Å. In the third Li1+ site, Li1+ is bonded in a 3-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.66 Å. In the fourth Li1+ site, Li1+ is bonded in a 3-coordinate geometry to seven O2- atoms. There are a spread of Li–O bond distances ranging from 2.06–2.76 Å. In the fifth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 2.01–2.57 Å. In the sixth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.71 Å. In the seventh Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.97–2.60 Å. In the eighth Li1+ site, Li1+ is bonded in a 3-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.56 Å. In the ninth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 2.12–2.51 Å. In the tenth Li1+ site, Li1+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Li–O bond distances ranging from 2.03–2.84 Å. In the eleventh Li1+ site, Li1+ is bonded in a 5-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.98–2.37 Å. In the twelfth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 2.00–2.22 Å. There are six inequivalent V+3.33+ sites. In the first V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.93–2.10 Å. In the second V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.98–2.08 Å. In the third V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.97–2.08 Å. In the fourth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.98–2.06 Å. In the fifth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.95–2.07 Å. In the sixth V+3.33+ site, V+3.33+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.96–2.08 Å. There are two inequivalent Mn2+ sites. In the first Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.93–2.19 Å. In the second Mn2+ site, Mn2+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.91–2.15 Å. There are twelve inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 17–53°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with four VO6 octahedra. The corner-sharing octahedra tilt angles range from 18–47°. There are a spread of P–O bond distances ranging from 1.52–1.56 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 27–47°. There are a spread of P–O bond distances ranging from 1.53–1.57 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 28–47°. There are a spread of P–O bond distances ranging from 1.53–1.56 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 16–48°. There is two shorter (1.53 Å) and two longer (1.56 Å) P–O bond length. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 29–46°. There are a spread of P–O bond distances ranging from 1.54–1.57 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 29–47°. There are a spread of P–O bond distances ranging from 1.54–1.58 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 25–46°. There are a spread of P–O bond distances ranging from 1.53–1.56 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 23–47°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 30–47°. There is two shorter (1.54 Å) and two longer (1.57 Å) P–O bond length. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and corners with two MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–51°. There is three shorter (1.54 Å) and one longer (1.56 Å) P–O bond length. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with four VO6 octahedra. The corner-sharing octahedra tilt angles range from 23–48°. There are a spread of P–O bond distances ranging from 1.53–1.56 Å. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the second O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the third O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the sixth O2- site, O2- is bonded in a distorted linear geometry to one V+3.33+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the ninth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted trigonal pyramidal geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted trigonal pyramidal geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twentieth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn2+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a distorted trigonal pyramidal geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one V+3.33+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted rectangular see-saw-like geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twenty-eighth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one V+3.33+, and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one Mn2+, and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the thirty-eighth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn2+, and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn2+ and one P5+ atom. In the fortieth O2- site, O2- is bonded in a distorted T-shaped geometry to one Li1+, one V+3.33+, and one P5+ atom. In the forty-first O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the forty-second O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V+3.33+, and one P5+ atom. In the forty-third O2- site, O2- is bon